Detrimental hot weather conditions include: • High ambient temperature. • High concrete temperature. • Low relative humidity. • High wind speed. • Solar radiation.
Difficulties in Hot Weather • Increased water demand. • Accelerated slump loss. • Increased rate of setting. • Increased tendency of plastic shrinkage cracking. • Critical need for prompt early curing.
Hot Weather Concreting • Certain precautions should be taken in order to reduce the difficulties in hot weather conditions. • Temperature ranging from 10 to 15˚C is desirable, but such temperatures are not always practical. • Many specifications require that concrete when placed should have a temperature of less than 29 to 32˚C.
Precautions Depends on • Type of construction. • Characteristics of the materials being used. • The experience of placing and finishing crew in dealing with the atmospheric conditions in the site.
Precautions • Use materials and mix proportions that have a good record in hot weather conditions. • Cool the concrete or one or more of its ingredients. • Use a concrete consistency that allows rapid placement and consolidation. • Reduce the time of transporting, placing, and finishing as possible. • Schedule concrete placements to avoid extreme weather, such as at night or during favorable weather conditions. • Consider the methods to limit moisture loss during placing and finishing such as sunshades, wind screens, fogging, and spraying.
Effect of High Concrete Temperature • As concrete temperature increases there is a loss in slump that is often unadvisedly compensated for by adding water to the concrete at the jobsite. At higher temperatures a greater amount of water is required to hold slump constant than is needed at lower temperatures.
Effect of High Concrete Temperature • increase the rate of setting and shorten the length of time within which the concrete can be transported, placed, and finished. • Setting time can be reduced by 2 or more hours with a 10°C increase in concrete temperature
Effect of High Concrete Temperature • There is an increased tendency for cracks to form both before and after hardening. • Rapid evaporation of water from freshly placed concrete can cause plastic-shrinkage cracks before the surface has hardened. • Cracks may also develop in the hardened concrete because of increased drying shrinkage due to higher water contents or thermal volume changes as the concrete cools.
Effect of High Concrete Temperature • High initial concrete temperatures has significant effect on compressive strength. The concrete temperatures at the time of mixing, casting, and curing were 23°C, 32°C, 41°C, and 49°C. After 28 days, the specimens were all moist-cured at 23°C until the 90-day and one-year test ages.
Cooling Concrete Materials • Lower the temperature of concrete materials before mixing. • The contribution of each material is related to • Temperature. • Specific heat. • Quantity of each material.
Where T = temperature of the freshly mixed concrete, °CelsiusTa, Tc, Tw, and Twa = temperature (°Celsius) of aggregates, cementing materials, added mixing water, and free water on aggregates, respectively
Supplementary Cementitious Materials • The use of supplementary materials (fly ash, ground granulated blast furnace slag) can help in hot weather conditions. • These material slow the rate of setting as well as the rate of slump loss.
Preparation Before Placing • Mixers, chutes, conveyor belts, hoppers, pump lines, and other equipments for handling concrete should be shaded, painted white, or covered with wet burlap to reduce solar heat. • Forms, reinforcing steel, and subgrade should be fogged or sprinkled with cool water just before concrete is placed. • Restrict placement of concrete to early morning, evening, or night time hours, especially in arid climates. This will help in minimizing thermal shrinkage and cracking of thick slabs and pavements.
Transporting, Placing, and Finishing • Should be done as quickly as practical during hot weather. • Delays contribute to the loss of slump and increase in concrete temperature. • Prolonged mixing should be avoided. • If delays occur, stopping mixer and then agitating can minimize the heat generated by mixing.
Transporting, Placing, and Finishing • Setting of concrete is more rapid in hot weather. • Extra care must be taken with placement techniques to avoid cold joints. • Temporary sunshades and windbreaks help to minimize cold joints.
Plastic Shrinkage Cracking • Associated with hot-weather concreting, • It can occur any time ambient conditions produce rapid evaporation of moisture from the concrete surface. • These cracks occur when water evaporates from the surface faster than it can rise to the surface during the bleeding process. • Rapid drying shrinkage creates tensile stresses in the surface that often result in short, irregular cracks.
Plastic Shrinkage Cracking • Plastic shrinkage cracking increases with: 1. Low air temperature2. High concrete temperature3. Low humidity4. High wind speed
Length ranges from 5 to 100 cm Spaced in an irregular pattern from 5 to 60 cm
Plastic Shrinkage Cracking • When the rate of evaporation exceeds 1 kg/m2 per hour, precautionary measures such as windscreens are required around all sides of concrete elements. • With concrete mixtures containing pozzolans, cracking is possible if the rate of evaporation exceeds 0.5 kg/m2 per hour. • Concrete containing silica fume is particularly prone to plastic shrinkage because bleeding rates are commonly only 0.25 kg/m2 per hour.
Precautions to Minimize Plastic Shrinkage Cracking • Moisten concrete aggregates that are dry and absorptive. • Keep the concrete temperature low by cooling aggregates and mixing water. • Dampen the subgrade (Fig. 13-9) and fog forms prior to placing concrete. • Erect temporary windbreaks to reduce wind velocity over the concrete surface. • Erect temporary sunshades to reduce concrete surface temperatures.
Precautions to Minimize Plastic Shrinkage Cracking 6. Protect the concrete with temporary coverings, such as polyethylene sheeting, during any appreciable delay between placing and finishing. 7. Fog the slab immediately after placing and before finishing, taking care to prevent the accumulation of water that may reduce the quality of the cement paste in the slab surface. 8. Add plastic fibers to the concrete mixture to help reduce plastic shrinkage crack formation.
Methods to Minimize Plastic Drying Shrinkage • Use of a fog spray will raise the relative humidity of the ambient air over the slab, thus reducing evaporation from the concrete. • Fog nozzles atomize water using air pressure. • Spray application of temporary moisture-retaining films (usually polymers). • Reduction of time between placing and the start of curing by eliminating delays during construction.
Curing in Hot Weather • The need for moist curing of concrete slabs is greatest during the first few hours after finishing. • To prevent the drying of exposed concrete surfaces, moist curing should commence as soon as the surfaces are finished. • When the air temperature is at or above 27°C, curing during the basic curing period should be accomplished by water spray or by using saturated absorptive fabric
Curing in Hot Weather • For mass concrete, curing should be by water for the basic curing period when the air temperature is at or above 20°C, in order to minimize the temperature rise of the concrete. • If approved, the application of the curing compound should be preceded by 24 hours of moist curing. • Crazing cracks are very fine and barely visible except when the concrete is drying after the surface has been wet. They do not penetrate much below the surface.
Admixtures • A retarding admixtures can be very helpful in delaying the setting time, despite increased rate of slump loss resulting from their use. • A hydration control admixture can be used to stop cement hydration and setting. As a general rule a 5°C to 9°C temperature rise per 45 kg of Portland cement can be expected from the heat of hydration.